Available online at www.sciencedirect.com
Physica E 18 (2003) 202 – 205 www.elsevier.com/locate/physe
Transport in nanostructures and nanotubes Tsuneya Ando∗ , Hidekatsu Suzuura Department of Physics, Tokyo Institute of Technology, 2-12-1 Ookayama, Meguro-ku, Tokyo 152-8551, Japan
Abstract In two-dimensional honeycomb lattices, electronic states are described by Weyl’s equation for a massless neutrino when each site is occupied by an electron on average. The system has a topological singularity at the origin k = 0 of the wave vector, giving rise to nontrivial Berry’s phase when k is rotated around the origin. The singularity causes discrete jumps in the conductivity at the energy corresponding to k = 0 in honeycomb lattices and leads to the absence of backscattering and a perfect conductance in carbon nanotubes. ? 2002 Elsevier Science B.V. All rights reserved. Keywords: Honeycomb lattice; Topological singularity; Berry’s phase; Anomaly
Since the discovery of carbon nanotubes , the transport property of the carbon network of the nanometer scale has attracted much attention. A carbon nanotube consists of coaxially rolled two-dimensional (2D) graphite sheets having a honeycomb lattice. A honeycomb lattice can be realized at semiconductor heterostructures with hexagonal antidot arrays. In this paper a review of e8ects a topological singularity present in the Schr9odinger equation on transport properties of such honeycomb lattices and also of carbon nanotubes is given. In a honeycomb lattice, a unit cell contains two carbon atoms denoted by A and B as shown in Fig. 1. Two bands having approximately a linear dispersion cross the Fermi level at K and K points of the
Corresponding author. E-mail address: [email protected]
with vanishing rest mass and constant velocity independent of the wave vector. It is known that a neutrino has a helicity and its spin is quantized into the direction of its motion. In fact, in the absence of a magnetic
where L2 is the system area, ’(k) is the angle of the wave vector k = (kx ; ky ), k = |k|, and s = +1 and −1 for the conduction and valence bands, respectively. The velocity is given by |v| = =˝ independent of k and . The density of states becomes D() = ||=22 , which varies linearly as a function of the energy and vanishes at = 0. Fig. 2 shows the energy dispersion and the density of states of the system described by Eq. (1). The above wave function acquires Berry’s phase − when the wave vector k is rotated around the origin, although it looks continuous as a function of k [4,5]. This is equivalent to the well-known signature change of the spinor wave function or a spin rotation operator under a 2 rotation. It should be noted that ’ = − when the closed contour encircles the origin k=0 but ’=0 when the contour does not contain k=0. Further, the wave function at k=0 depends on the direction of k and its “spin” direction is unde
1386-9477/03/$ - see front matter ? 2002 Elsevier Science B.V. All rights reserved. doi:10.1016/S1386-9477(02)00966-9
T. Ando, H. Suzuura / Physica E 18 (2003) 202 – 205
Fig. 1. The structure of a honeycomb lattice. A unit cell contains two atoms denoted as A and B (small circles). A honeycomb lattice can be realized at a semiconductor heterostructure by fabrication of a short-period hexagonal antidot array (shadowed big circles).
conductivity 0 = (e2 =22 ˝)W −1 independent of the Fermi level, i.e., nonzero even at = 0 where the density of states vanishes. In the presence of a magnetic
with = x; y and = x; y is given by xx = yy = 0 =[1 + (!c )2 ] and xy = − yx = − 0 !c =[1 + (!c )2 ]. Using the explicit expressions for !c and , we have √xx = 0 4 =(1 + 4 ) and xy = − 0 2 =(1 + 4 ), with = 2W (F =B ), where B is the magnetic energy de
iF e2 4 +1 8˝ ˝! + i[˝=(F )]
Fig. 2. The energy dispersion and density of states in the vicinity of the Fermi level in a honeycomb lattice.
facts show the presence of a topological singularity at k = 0. This topological singularity causes a zero-mode anomaly in the conductivity of the honeycomb lattice and also the absence of backscattering in metallic carbon nanotubes as will be demonstrated below. A singularity at = 0 manifests itself in magnetic
˝! + i[˝=(˝!=2)] − 2F i : ln ˝! + i[˝=(˝!=2)] + 2F
Because ˝=() ˙ ||, the frequency dependence is scaled by ˝!=F . The scaling of the dynamical conductivity (˝!=F ) shows that (!; F ) exhibits a singular behavior at the point (!; F ) = (0; 0). The correct way is to let ! → 0 at each F , leading to a singular jump of the static conductivity to e2 =8˝ from 0 at F = 0. A more re
T. Ando, H. Suzuura / Physica E 18 (2003) 202 – 205
Conductivity (units of e 2/π 2 h)
εc /ε0 =50.0 SCBA Boltzmann
50.0 20.0 10.0
25 20 15 10 5 0 -2
Energy (units of ε0)
Fig. 3. An example of the conductivity vs the Fermi energy. The solid lines represent the conductivity calculated in SCBA and horizontal dotted lines the corresponding Boltzmann result. 0 is an arbitrary energy scale (after Ref. ).
tight-binding model. They can be well reproduced in the k·p scheme discussed above . In the k·p scheme, electrons in a nanotube can be regarded as neutrinos on a cylinder surface with a
tubes, on the other hand, backscattering appears because the symmetry is destroyed by a nonzero AB magnetic Lux. An important information has been obtained on the effective mean free path in nanotubes by single-electron tunneling experiments [22,23]. The Coulomb oscillation in semiconducting nanotubes is quite irregular and can be explained only if nanotubes are divided into many separate spatial regions in contrast to that in metallic nanotubes . This behavior is consistent with the presence of considerable amount of backward scattering leading to a strong localization of the wave function. In metallic nanotubes, the wave function is extended in the whole region of a nanotube because of the absence of backward scattering. With the use of electrostatic force microscopy the voltage drop in a metallic nanotube has been shown to be negligible in comparison with an applied voltage . At nonzero temperatures, lattice vibrations usually constitute the major source of electron scattering and limit the resistivity. Usually long-wavelength acoustic phonons are most important. These modes can be described by a continuum model [26–28]. An acoustic phonon gives rise to an e8ective electron–phonon coupling called the deformation potential V1 = g1 (uxx + uyy ) with uxx = (@ux =@x) + (uz =R) and uyy = @uy =@y, where ux , uy , and uz represent lattice displacements in the x, y, and z directions, respectively. This potential appears as a diagonal term. A very rough estimation gives g1 ∼ 30 eV. Phonon cause also a change in the distance between neighboring carbon atoms. This gives rise to an o8-diagonal elements V2 = g2 e3i" (uxx − uyy + 2iuxy ) with g2 = (3(=4)0 , where −0 is the transfer between nearest neighbors, ( = −d ln 0 =d ln b, b is the bond length, and is a quantity smaller than unity dependent on microscopic models of phonons. Usually, we have ( ∼ 2 (see, for example, Ref. ) and ∼ 1=3, which give g2 ∼ 0 =2 or g2 ∼ 1:5 eV. This coupling constant is much smaller than the deformation potential. It corresponds to one given by Kane and Mele  without the reduction factor . The diagonal term does not contribute to the backscattering as in the case of impurities and only the much smaller o8-diagonal term has some contribution. The mean free path * is estimated as * = (a2 =3kB T2 (2 )L, where L = |L|, is the shear modulus of 2D graphite, and a is the lattice constant. We obtain * ∼ 600L at room temperature, which is larger than 1 m for thin armchair nanotubes with diameter ∼ 1:5 nm and increases in proportion to L. This shows that a metallic CN is ballistic even at room temperature. The situation changes dramatically when other bands start to be occupied. Fig. 4 shows the Fermi energy dependence of the conductivity obtained by solving Boltzmann equation . In summary, in 2D honeycomb lattices the topological singularity present at k = 0 gives rise to nontrivial Berry’s phase of the wave function when the k is rotated around the origin. This singularity gives rise to discrete jumps in the Boltzmann conductivity at the energy corresponding to k = 0. This jump is somewhat smoothed out but prevails
T. Ando, H. Suzuura / Physica E 18 (2003) 202 – 205 g1/g2=10 Metal Semiconductor
Fig. 4. The Fermi-energy dependence of the conductivity for metallic (solid line) and semiconducting (broken line) CN’s with g1 =g2 = 10 in units of A (0) denoting the conductivity of an armchair CN with F = 0. After Ref. .
practically even if level broadening e8ects are properly taken into account in the SCBA. In carbon nanotubes, this topological singularity leads to the absence of backscattering and a perfect conductance even in the presence of scatterers. Phonons cause backscattering at high temperatures, but effects are very weak and nanotubes are considered as ballistic conductors even at room temperature, because the strong deformation potential has no contribution. This work has been supported in part by Grants-in-Aid for COE (12CE2004 “Control of Electrons by Quantum Dot Structures and Its Application to Advanced Electronics”) and Scienti
S. Iijima, Nature (London) 354 (1991) 56. J.C. Slonczewski, P.R. Weiss, Phys. Rev. 109 (1958) 272. H. Ajiki, T. Ando, J. Phys. Soc. Jpn. 62 (1993) 1255. M.V. Berry, Proc. Roy. Soc. London A 392 (1984) 45. T. Ando, T. Nakanishi, R. Saito, J. Phys. Soc. Jpn. 67 (1998) 2857.  Y. Zheng, T. Ando, Phys. Rev. B 65 (2002) 245420.  T. Ando, T. Nakanishi, J. Phys. Soc. Jpn. 67 (1998) 1704.
 T. Ando, Y. Zheng, H. Suzuura, J. Phys. Soc. Jpn. 71 (2002) 1318.  N.H. Shon, T. Ando, J. Phys. Soc. Jpn. 67 (1998) 2421.  H. Ajiki, T. Ando, J. Phys. Soc. Jpn. 62 (1993) 2470 [Errata, J. Phys. Soc. Jpn. 63 (1994) 4267].  H. Ajiki, T. Ando, Physica B 201 (1994) 349; H. Ajiki, T. Ando, Jpn. J. Appl. Phys. 34-1 (Suppl) (1995) 107.  T. Ando, J. Phys. Soc. Jpn. 66 (1997) 1066.  N.A. Viet, H. Ajiki, T. Ando, J. Phys. Soc. Jpn. 63 (1994) 3036.  H. Suzuura, T. Ando, in: N. Miura, T. Ando (Eds.), Proceedings of the 25th International Conference on the Physics of Semiconductors, Springer, Berlin, 2001, p. 1525.  H. Ajiki, T. Ando, J. Phys. Soc. Jpn. 64 (1995) 260; H. Ajiki, T. Ando, J. Phys. Soc. Jpn. 65 (1996) 2976.  H. Ajiki, T. Ando, J. Phys. Soc. Jpn. 64 (1995) 4382.  T. Ando, J. Phys. Soc. Jpn. 69 (2000) 1757.  H. Matsumura, T. Ando, J. Phys. Soc. Jpn. 67 (1998) 3542; H. Matsumura, T. Ando, J. Phys. Soc. Jpn. 70 (2001) 2401; H. Matsumura, T. Ando, Mol. Cryst. Liq. Cryst. 340 (2000) 725; H. Matsumura, T. Ando, in: N. Miura, T. Ando (Eds.), Proceedings of 25th International Conference on the Physics of Semiconductors, Springer, Berlin, 2001, p. 1655.  H. Matsumura, T. Ando, J. Phys. Soc. Jpn. 70 (2001) 2657.  T. Yaguchi, T. Ando, J. Phys. Soc. Jpn. 70 (2001) 3641; T. Yaguchi, T. Ando, J. Phys. Soc. Jpn. 71 (2002) 2224.  T. Nakanishi, T. Ando, J. Phys. Soc. Jpn. 68 (1999) 561.  S.J. Tans, M.H. Devoret, H. Dai, A. Thess, R.E. Smalley, L.J. Geerligs, C. Dekker, Nature (London) 386 (1997) 474.  A. Bezryadin, A.R.M. Verschueren, S.J. Tans, C. Dekker, Phys. Rev. Lett. 80 (1998) 4036.  P.L. McEuen, M. Bockrath, D.H. Cobden, Y.-G. Yoon, S.G. Louie, Phys. Rev. Lett. 83 (1999) 5098.  A. Bachtold, M.S. Fuhrer, S. Plyasunov, M. Forero, E.H. Anderson, A. Zettl, P.L. McEuen, Phys. Rev. Lett. 84 (2000) 6082.  H. Suzuura, T. Ando, Physica E 6 (2000) 864.  H. Suzuura, T. Ando, Mol. Cryst. Liq. Cryst. 340 (2000) 731.  H. Suzuura, T. Ando, Phys. Rev. B 65 (2002) 235412.  W.A. Harrison, Electronic Structure and the Properties of Solids, W.H. Freeman and Company, San Francisco, 1980.  C.L. Kane, E.J. Mele, Phys. Rev. Lett. 78 (1987) 1932.